- Nano Express
- Open Access
Double Morphology of Co9S8 Coated by N, S Co-doped Carbon as Efficient Anode Materials for Sodium-Ion Batteries
Nanoscale Research Letters volume 15, Article number: 19 (2020)
Co9S8 is a potential anode material for its high sodium storage performance, easy accessibility, and thermostability. However, the volume expansion is a great hindrance to its development. Herein, a composite containing Co9S8 nanofibers and hollow Co9S8 nanospheres with N, S co-doped carbon layer (Co9S8@NSC) is successfully synthesized through a facile solvothermal process and a high-temperature carbonization. Ascribed to the carbon coating and the large specific surface area, severe volume stress can be effectively alleviated. In particular, with N and S heteroatoms introduced into the carbon layer, which is conducive to the Na+ adsorption and diffusion on the carbon surface, Co9S8@NSC can perform more capacitive sodium storage mechanism. As a result, the electrode can exhibit a favorable reversible capacity of 226 mA h g−1 at 5 A g−1 and a favorable capacity retention of 83.1% at 1 A g−1 after 800 cycles. The unique design provides an innovative thought for enhancing the sodium storage performance.
With the rapid development of power reserve systems in electric vehicles and portable electronic products, sodium-ion batteries (SIBs) have become a strong competitor to lithium-ion batteries (LIBs), because of the similar charge-discharge behavior to LIBs, low cost, and vast natural reserves [1,2,3]. And the electrochemical potential of Na (− 2.71 V vs the standard hydrogen electrode, SHE) is higher than that of Li (− 3.04 V) with 330 mV, which makes SIBs possible to meet large-scale energy storage demands [4,5,6]. However, the most important challenge in SIBs is the large volume expansion during the process of sodiation originated from the great strain derived from the larger radius of Na+ (1.02 Å) than Li+ (0.76 Å) [7, 8]. This will result in severe pulverization and exfoliation of active materials from copper foil and further lead to poor cycling performance. Therefore, rational design of anode materials is an impending concern.
Diverse anode materials have been reported for their high theoretical capacity, such as transition-metal sulfides (TMSs) [9,10,11,12,13,14], transition-metal oxides (TMOs) [15,16,17,18], phosphides [19,20,21,22], and carbon composites [23,24,25,26]. Among them, cobalt-based MSs (such as CoS, CoS2, Co3S4, and Co9S8) have attracted great attention for its near-metallic conductivity and easy accessibility [27,28,29]. Specifically, cubic Co9S8 attracts much attention for its great thermostability. Unfortunately, it is still impeded by the severe volume variation, slow Na+ diffusion rate, and poor conductivity [30,31,32]. Great efforts have been made to handle the shortcomings of Co9S8.
So far, most studies have also focused on designing novel carbon materials with heteroatom (N, P, S, B) doped, such as sandwich-like structures with N, S-doped RG O[33, 34], nanoflower-like N-C/CoS 2, Co9S8 coated with N-doped carbon nanospheres [36, 37], and N, S-doped nanofibers [38, 39]. Carbon coating can not only enhance the conductivity of TMSs, but also remit the stress stemming from the volume expansion. In particular, with the heteroatom doping, the electronic structure of carbon can be modified to improve the physical and chemical properties by generating extrinsic defects, expanding the interlayer distance and offering additional electron transfer route when heteroatoms are bonded with carbon atoms [40,41,42,43,44].
Herein, we synthesize double morphology of Co9S8, containing nanofibers and hollow nanospheres, both coated with N, S co-doped carbon (denoted as Co9S8@NSC), for highly stable SIBs. Nanofiber-like structure provides long-range continuous electron transport, while the hollow nanospheres enhance the infiltration of electrolyte. The N, S co-doped carbon layer can provide more free electrons, which benefit the adsorption of Na+ on the surface and enhance the integral conductivity. Due to the hardness of carbon coating and 3D network, volume variation during sodium ion insertion/extraction can be well alleviated from atomic and 3D level. And the high specific surface area can enhance the capacity of pseudo-capacitance contribution, leading to excellent rate performance. As a result, SIBs with Co9S8@NSC can deliver a stable capacity retention of 318 mA h g−1 after 800 cycles at 1 A g−1 with the coulombic efficiency of ~ 100%, making it a promising anode for large-scale SIBs.
Synthesis of Co9S8@NSC
In a typical process, the composites were prepared by coaxial electrospinning following alcohol-thermal method and carbonization.
Preparation of Electrospun Nanofibers
0.74 g PAN (Sigma-Aldrich, MW = 150,000) and 9 ml DMF was stirred for overnight to form the homogeneous outer solution, while 1.8 g Cobalt(II) acetylacetonate (Co(acac)2, Aladdin, purity ≥ 99%) and 0.74 g PAN (Macklin, MW = 150000) were mixed with 9 ml DMF and stirred at the same time as the dark red inner solution. Then, the two kinds of solutions were conducted by coaxial electrospinning (needle size: inner 17 G, outer:22 G). The distance between the needle and Al foil collector was 15 cm, and the condition temperature was maintained at 65 °C. Then, electrical potential was applied at 15 kV with flow rate of two syringes both at 1.5 ml h−1. The final precursor fibers were dried at 60 °C in vacuum for 24 h.
Sulfuration and Carbonization
The obtained nanofibers were firstly mixed with 50 ml ethanol containing thioacetamide (TAA, Aladdin, purity ≥ 99%) in 100 ml Teflon-lined stainless-steel autoclave at 120 °C for 6 h by solvothermal method. The final product was obtained by carbonizing at 700 °C for 1 h with a heating rate of 5 °C min−1 and cooling down naturally. For comparison, sample without cobalt (N, S co-doped carbon, denoted as NSC) was also prepared using the same method mentioned above without adding Co(acac)2.
The morphology and structure of the Co9S8@NSC were characterized by scanning electron microscopy (SEM, ZEISS Gemini 500) and transmission electron microscopy (TEM, JEM-2100HR). Thermal gravity analysis (TGA) test was performed to evaluate the content of Co9S8 by Netzsch STA449. The crystalline structures and surface valence state analyses were detected by X-ray photoelectron spectroscopy (XPS, ESCALAB 250Xi), X-ray powder diffraction (XRD, Bruker D8 Advance), and Raman spectra. The specific surface area and pore size distribution were recorded from the Brunauer-Emmett-Teller (BET, Micromeritics ASAP-2020) analysis instrument.
Slurries were obtained by mixing active materials, poly (vinylidene fluoride) (PVDF), and Super P (weight ratio of 8:1:1) with N-methylpyrrolidone (NMP). Then, the working electrode was prepared by coating the slurries uniformly on a precut copper foil (diameter 12 mm) and dried at 60 °C in air and vacuum overnight, respectively. The CR2032-type coin cells were assembled with sodium metal as the reference electrode, glass fiber membrane as the separator, and the as-prepared copper foil as the anode. The electrolyte was 1 M NaClO4 in EC/DMC (EC:DMC = 1:1, in volume) with 5.0% FEC. The assembly procedures were all carried out in an Ar-filled glove box (O2 < 0.1 ppm, H2O < 0.1 ppm). The cyclic voltammetry (CV) and electrochemical impedance spectroscopy (EIS) results were obtained from an electrochemical workstation (CHI660E, Shanghai Chen Hua Instruments Ltd). And the galvanostatic discharge-charge tests were conducted in a NEWARE battery testing system.
Results and Discussion
The synthesis process of Co9S8@NSC is illustrated in Additional file 1: Scheme S1, including coaxial electrospinning, solvothermal sulfuration, and carbonization. The crystallinity of Co9S8@NSC and NSC after those procedures is shown in Fig. 1a. The XRD curve of Co9S8@NSC displays typical characteristic diffraction peaks in accord with the cubic Co9S8 phase (JCPDS no. 86-2273), while NSC only exhibits peaks of hard carbon. The broad peak at 24.8° is corresponding to (111) plane of amorphous carbon. Strikingly, it is lower than the standard value of 26.6°, indicating expanded interlayer distance and lower graphitization derived from N, S co-doped sites into the carbon . The Raman spectra (Fig. 1b) also confirms the existence and composition of carbon in the composites. Co9S8@NSC and NSC both exhibit two obvious peaks of 1308 cm−1 and 1513 cm−1, representing the D band and G band of carbon, respectively. Besides, Co9S8@NSC owns a weak typical peak located at 671 cm−1, corresponding to the Co9S8. In detail, the D band is attributed to the structure defects of amorphous carbon, while the G band is due to the E2g vibration mode of Sp2 bond between graphitic carbon atoms . The slightly larger ID/IG of Co9S8@NSC (1.31) than NSC (1.14) indicates more defects exist in the composites, resulted from N doping and S doping.
The weight ratio of Co9S8 is measured by thermogravimetric analysis (TGA) as shown in Fig. 1c. After heating to 700 °C in air with 10 °C min−1, multistep reaction is involved with the final product as Co3O4, which can be ascribed to: (1) the evaporation of trace water (below 100 °C), (2) the oxidation of Co9S8 to CoSOx (from 200 to 400 °C), and (3) the decomposition of carbon and continuous oxidation of CoSOx (above 400 °C). According to these reactions, the content of Co9S8 in the composites is calculated as 40.1%. Co9S8@NSC exhibits typical type IV isotherm curves, indicating the mesoporous structure, while the NSC is microporous (Fig. 1d). The specific surface area of Co9S8@NSC (122.5 m2 g−1) is much larger than NSC (4.1 m2 g−1), which can benefit the infiltration of electrolyte for fast insertion/extraction of Na+ and remit the severe volume change. The pores of Co9S8@NSC with average size of 8.6 nm (shown in Additional file 1: Figure S1) are derived from the pyrolysis of chemical groups of polyacrylonitrile, dissolution of Co(acac)2 from the nanofibers, and the formation of hollow Co9S8 nanospheres.
X-ray photoelectron spectroscopy (XPS) is conducted to identify the chemical composition of Co9S8@NSC. The signals in the survey spectrum are accord with five elements of C, N, O, S, and Co in Fig. 2a. The presence of O should be due to the exposure of the sample in air with some oxygen adsorbed on the surface. The high-resolution spectrum of C 1s (Fig. 2b) displays four peaks, which are located at 284.6 eV (C-C/C=C), 285.0 eV (C-N), 285.8 eV (C-S), and 288.6 eV (C=N) . The Co 2p spectrum was shown in Fig. 2c. Peaks located at 786.1 eV and 803 eV can be fitted to the satellite peaks of Co 2p3/2 and Co 2p1/2, respectively. In addition, peaks of 778.5 eV and 793.6 eV and another two peaks at 781.4 eV and 797.2 eV belong to Co2+ and Co3+, respectively . Furthermore, the S 2p spectrum (Fig. 2d) is fitting into four peaks, consisting of 162.45 eV (S-Co), 163.7 eV (S-C), 165 eV (S-C), and 168.2 eV (sulfate) . And N 1s spectra (Additional file 1: Figure S2) contain three peaks at 398.4 eV, 400.1 eV, and 401.0 eV, which correspond to pyridinic N, pyrrolic N, and graphitic N, respectively . Compared to the alone carbon materials, introducing N,S co-doped carbon sites can provide more free electrons, which benefits the adsorption of Na+ on the surface and enhances the integral conductivity . The results of all XPS spectrums confirm the presence of N, S co-doping in Co9S8@NSC.
The interesting morphologies and detailed internal structures of Co9S8@NSC and NSC are measured by SEM and TEM. Figure 3a–c depicts the Co9S8@NSC consist of two kinds of structure including hollow nanospheres and nanofibers. These nanofibers are composed by carbonization of PAN fibers. The formation of nanospheres adhered on the nanofibers may be attributed to the decomposition and sulfurization of Co(acac)2 which was dissolved from the inside of PAN electrospinning fibers. And the composites own the distinctly coarse surface, which can enhance the wettability of electrolyte. Additional file 1: Figure S3a–c displays the NSC morphology with only smooth nanofibers cemented to each other without nanospheres, which can be due to the absence of Co-based compound and melt of PAN nanofibers in the process of carbonization. The elemental composition is confirmed by EDS mapping (Additional file 1: Figure S4), with C, N, Co, and S elements uniformly distributing in the composites. And this further demonstrates the successful doping of N, S element.
As displayed in Fig. 3d–f, TEM images reveal the internal details of the morphologies of Co9S8@NSC. Figure 3d and e show the Co9S8 nanoparticles are embedded in carbon nanofibers and hollow nanospheres, which confirms the point proposed above about the formation of the hollow nanospheres. Figure 3f reveals the interplanar distance of 0.308 nm, matching well with the (311) planes of Co9S8, while the NSC in Additional file 1: Figure S3d–f manifests the traditional character of hard carbon. Co9S8 nanoparticles with size all bellowing 50 nm distribute uniformly in the composite, and the thickness of carbon coating layer is measured 3–5 nm (Fig. 3f). Owing to the rough surface, hollow structure, and carbon coating, severe pulverization and exfoliation of active materials resulting from volume variation might be alleviated effectively.
To investigate the electrochemical performance of Co9S8@NSC, 2032-type coin cells are assembled for electrochemical tests. As shown in Fig. 4a, the CV curves of Co9S8@NSC record the initial five cycles at a scan rate of 0.1 mV s−1. The first cycle is far different from the subsequent cycles with a broad peak at 0.476 V in cathodic sweep, which is assigned to the formation of solid electrolyte interface (SEI) film, irreversible intercalation of Na+, and the stepwise conversion of Co9S8 to Co and Na2S . In the first anodic sweep, two oxidation peaks of 0.375 V and 1.682 V can be attributed to the multistep reaction of Co to CoSx . The following CV curves of Co9S8@NSC are gradually overlapped, indicating the high electrochemical reversibility. For comparison, CV curves of NSC in Additional file 1: Figure S5a show the typical characteristic peaks of carbon, which represents the adsorption and insertion of Na+ in carbon nanofibers. Figure 4b and Additional file 1: Figure S5b display the charge/discharge curves for different cycles of Co9S8@NSC and NSC with the initial coulombic efficiency (CE) of 54.1% and 28.3%, respectively. The relatively low CE is caused by the irreversible formation of SEI film and electrolyte consumption . The curves of these two samples manifest distinctive voltage platform of Co9S8 and carbon, which are in accord with the results of CV tests (Fig. 4a and Additional file 1: Figure S5a).
Rate performance is shown in Fig. 4c. The capacity of Co9S8@NSC can reach 226 mAh g−1 at 5 A g−1, while NSC can only maintain 21 mAh g−1. And then, when the current density recovers to 100 mAh g−1, the capacity can be well returned to 440 mAh g−1. Figure 4d shows the cycling performance of Co9S8@NSC. The discharge capacities of Co9S8@NSC maintain at 423 mAh g−1 at 200 mA g−1 and 318 mAh g−1 at 1 A g−1 after 800 cycles with initial coulombic efficiency at 42.3% and 37.4%, respectively. This can be explained by the reaction mechanism transformation from intercalation/deintercalation at low current density to adsorption/desorption of Na+ at high current density . Apparently, the capacities of Co9S8@NSC are all higher than those of NSC, which is due to the more active sites derived from Co9S8 and N, S co-doping. In addition, the capacity retention of 87.4% at 200 mA g−1 and 83.1% at 1 A g−1 after 800 cycles indicate the stable cycling performance and benign reaction reversibility of Co9S8@NSC.
To understand the interfacial properties and internal resistances of Co9S8@NSC and NSC, electrochemical impedance spectra (EIS) has been conducted. As presented in Additional file 1: Figure S6a, the Nyquist plots of Co9S8@NSC after different cycles show typical semicircles in high-frequency region (charge transfer resistance, Rct) and an oblique line in low-frequency region (Warburg resistance, W). Before the initial cycle, the largest Rct (about 1600 Ω) of Co9S8@NSC is caused by insufficient infiltration of electrolyte. After 5 cycles, the Rct becomes very small as 153 Ω for the formation of SEI film and well contact with electrolyte. Furthermore, the decrease of the Rct can be also attributed to the process of activation of the Co9S8@NSC electrode interfacial. After 10 cycles, it almost keeps the same value, which indicates the excellent stability. For comparison, EIS of NSC is also investigated in Additional file 1: Figure S6b–e. The initial Rct of NSC is smaller than Co9S8@NSC, indicating the higher electroconductivity of NSC. As the cycle is going on, the Rct of Co9S8@NSC gradually becomes smaller than that of NSC, owing to the larger specific surface area and enough infiltration of electrolyte. These results mentioned above support the benign cycling and rate performance of Co9S8@NSC.
To gain further insight into the electrochemistry of Co9S8@NSC electrode, a kinetic analysis is conducted. The CV curves at different sweep rates from 0.1 to 0.9 mV s−1 are collected and shown in Fig. 5a. Varying from common ionic diffusion, the peak current (I, mA) is not completely linearly dependent to v1/2 (v is the scan rate, mV s−1), indicating the coexistence of non-faradic and faradic behaviors [35, 50]. And the results can be verified by the relation between log(I) and log(v), according to equation of log(I) = b log(v) + log(a). When the value of b reaches 0.5 or 1, it indicates that the reaction mechanism is totally controlled by ionic diffusion or capacitive behavior, respectively [51, 52]. As shown in Fig. 5b, the calculated values of b are 0.7518 (cathodic peak) and 0.7792 (anodic peak), which means more capacitive behavior.
Furthermore, the contribution of capacitive behavior can be obtained from the equation: i(V) = k1v + k2v1/2 , where i(V) is the current at a fixed voltage, v is the sweep rate, and k1v and k2v1/2 represent the capacitive capacity and ion diffusion capacity, respectively. When sweep rate is 0.5 mV s−1, the contribution ratio of the capacitive capacity reaches 69.2% (Fig. 5c). For different sweep rates, Fig. 5d illustrates an obvious tendency of the capacitive capacity ratio increasing with the scan rate from 0.1 to 0.9 mV s−1. The increasing capacitive contribution can be ascribed to high specific area and abundant active sites, which furthermore may be responsible for the excellent rate performance of the Co9S8@NSC electrode. All these results reveal a fast kinetic of Co9S8@NSC which resulted from the capacitive effect.
where n, A, and C represent the number of transferred electrons in the process of Na+ intercalation/deintercalation, the surface area, and the molar concentration of Na+, respectively. The DNa+ of Co9S8@NSC is proportional to the slope of the linear relations between Ip and v1/2 (Additional file 1: Figure S7). As a result, the slope values of anodic peak and cathodic peak of Co9S8@NSC are much positive and negative than those of NSC, respectively, which means that the DNa+ of Co9S8@NSC is much higher than NSC in the process of Na+ intercalation/deintercalation. In detail, it can be ascribed to favorable infiltration of electrolyte and much exposed active sites derived from the larger specific surface area of Co9S8@NSC.
In summary, a novel double morphology of Co9S8, containing hollow nanospheres and nanofibers, with coating N, S co-doped carbon layer has been successfully synthesized using coaxial electrospinning following sulfurization by solvothermal method and carbonization. Owing to the larger specific surface area and carbon coating, Co9S8@NSC can accommodate the volume change during the charge/discharge process. More uniformly, active sites derived from Co9S8 and N, S co-doped position can not only contact with much more electrolyte, but also accelerate diffusion of Na+ and reversible reaction between Na+ and Co9S8@NSC. When applied as anode materials, Co9S8@NSC can deliver a high reversible specific capacity of 318 mAh g−1 after 800 cycles at 1 A g−1 with the coulombic efficiencies remaining almost 100%, while the large surface area and abundant N, S co-doped sites can lead to the excellent rate capability. The study offers more possibilities of cobalt sulfides in designing effective anode materials for SIBs.
Availability of Data and Materials
All data used within this manuscript are available upon request.
- Co(acac)2 :
Cobalt(II) acetylacetonate hydrate
Electrochemical impedance spectroscopy
N, S co-doped carbon
Thermal gravity analysis
Hou H, Qiu X, Wei W, Zhang Y, Ji X (2017) Carbon anode materials for advanced sodium-ion batteries. Adv Energy Mater 7:1602898
Qiu S, Xiao L, Sushko ML, Han KS, Shao Y, Yan M, Liang X, Mai L, Feng J, Cao Y, Ai X, Yang H, Liu J (2017) Manipulating adsorption-insertion mechanisms in nanostructured carbon materials for high-efficiency sodium ion storage. Adv Energy Mater 7:1700403
Tan S, Jiang Y, Wei Q, Huang Q, Dai Y, Xiong F, Li Q, An Q, Xu X, Zhu Z, Bai X, Mai L (2018) Multidimensional synergistic nanoarchitecture exhibiting highly stable and ultrafast sodium-ion storage. Adv Mater 30:1707122
Chayambuka K, Mulder G, Danilov DL, Notten PHL (2018) Sodium-ion battery materials and electrochemical properties reviewed. Adv Energy Mater 8:1800079
Fu L, Wang X, Ma J, Zhang C, He J, Xu H, Chai J, Li S, Chai F, Cui G (2017) Graphene-encapsulated copper tin sulfide submicron spheres as high-capacity binder-free anode for lithium-ion batteries. ChemElectroChem. 4:1124–1129
Chen W, Lei T, Wu C, Deng M, Gong C, Hu K, Ma Y, Dai L, Lv W, He W, Liu X, Xiong J, Yan C (2018) Designing safe electrolyte systems for a high-stability lithium-sulfur battery. Adv Energy Mater 8:1702348
Zhang Y, Li X, Dong P, Wu G, Xiao J, Zeng X, Zhang Y, Sun X (2018) Honeycomb-like hard carbon derived from pine pollen as high-performance anode material for sodium-ion battery. ACS Appl Mater Interfaces 10:42796–42803
Ling L, Bai Y, Wang Z, Ni Q, Chen G, Zhou Z, Wu C (2018) Remarkable effect of sodium alginate aqueous binder on anatase TiO2 as high-performance anode in sodium ion batteries. ACS Appl Mater Interfaces 10:5560–5568
Jiang Y, Guo Y, Lu W, Feng Z, Xi B, Kai S, Zhang J, Feng J, Xiong S (2017) Rationally incorporated MoS2/SnS2 nanoparticles on graphene sheets for lithium-ion and sodium-ion batteries. ACS Appl Mater Interfaces 9:27697–27706
Jing M, Chen Z, Li Z, Li F, Chen M, Zhou M, He B, Chen L, Hou Z, Chen X (2018) Facile synthesis of ZnS/N,S co-doped carbon composite from zinc metal complex for high-performance sodium-ion batteries. ACS Appl Mater Interfaces 10:704–712
Liu ZM, Lu TC, Song T, Yu XY, Lou XW, Paik U (2017) Structure-designed synthesis of FeS2@C yolk-shell nanoboxes as a high-performance anode for sodium-ion batteries. Energy Environ Sci 10:1576–1580
Liu M-C, Li J, Yang Q-Q, Xu Y, Kong L-B, Bai R-J, Liu W-W, Niu W-J, Chueh Y-L (2019) Hierarchically interconnected Ni3S2 nanofibers as binder-free electrodes for high-performance sodium-ion energy-storage devices. ACS Appl Nano Mater 2:2634–2641
Wang H-E, Zhao X, Li X, Wang Z, Liu C, Lu Z, Zhang W, Cao G (2017) rGO/SnS2/TiO2 heterostructured composite with dual-confinement for enhanced lithium-ion storage. J Mater Chem A 5:25056–25063
Lei T, Chen W, Huang J, Yan C, Sun H, Wang C, Zhang W, Li Y, Xiong J (2017) Multi-functional layered WS2 nanosheets for enhancing the performance of lithium-sulfur batteries. Adv Energy Mater 7:1601843
Zhao C, Yu C, Zhang M, Huang H, Li S, Han X, Liu Z, Yang J, Xiao W, Liang J, Sun X, Qiu J (2017) Ultrafine MoO2-carbon microstructures enable ultralong-life power-type sodium ion storage by enhanced seudocapacitance. Adv Energy Mater 7:1602880
Wu Y, Jiang Y, Shi J, Gu L, Yu Y (2017) Multichannel porous TiO2 hollow nanofibers with rich oxygen vacancies and high grain boundary density enabling superior sodium storage performance. Small. 13:1700129
Ma D, Li Y, Mi H, Luo S, Zhang P, Lin Z, Li J, Zhang H (2018) Robust SnO2-x Nanoparticle-impregnated carbon nanofibers with outstanding electrochemical performance for advanced sodium-ion batteries. Angew Chem Int Ed 57:8901–8905
Wang HE, Zhao X, Yin K, Li Y, Chen L, Yang X, Zhang W, Su BL, Cao G (2017) Superior pseudocapacitive lithium-ion storage in porous vanadium oxides@C heterostructure composite. ACS Appl Mater Interfaces 9:43665–43673
Chen S, Wu F, Shen L, Huang Y, Sinha SK, Srot V, van Aken PA, Maier J, Yu Y (2018) Cross-linking hollow carbon sheet encapsulated CuP2 nanocomposites for high energy density sodium-ion batteries. ACS Nano 12:7018–7027
Feng S, Zhong H, Song J, Zhu C, Dong P, Shi Q, Liu D, Li J, Chang Y-C, Beckman SP, Song M-k, Du D, Lin Y (2018) Catalytic activity of Co–X (X = S, P, O) and its dependency on nanostructure/chemical composition in lithium–sulfur batteries. ACS Appl Energy Mater 1:7014–7021
Wang B, Wang G, Wang H, Bai J (2018) Hierarchically porous carbon nanofibers encapsulating carbon-coated mini hollow FeP nanoparticles for high performance lithium and sodium ion batteries. ChemNanoMat. 4:924–935
Shi S, Li Z, Sun Y, Wang B, Liu Q, Hou Y, Huang S, Huang J, Zhao Y (2018) A covalent heterostructure of monodisperse Ni2P immobilized on N, P-co-doped carbon nanosheets for high performance sodium/lithium storage. Nano Energy 48:510–517
Wu Z, Wang J, Song M, Zhao G, Zhu Y, Fu G, Liu X (2018) Boosting oxygen reduction catalysis with N-doped carbon coated Co9S8 microtubes. ACS Appl Mater Interfaces 10:25415–25421
Liu D, Hu A, Zhu Y, Zhou S, Duan Y, Tang Q, Deng W, Chen X (2019) Hierarchical microstructure of CNTs interwoven ultrathin Co3S4 nanosheets as a high performance anode for sodium-ion battery. Ceram Int 45:3591–3599
He P, Fang Y, Yu XY, Lou XWD (2017) Hierarchical nanotubes constructed by carbon-coated ultrathin SnS nanosheets for fast capacitive sodium storage. Angew Chem Int Ed 56:12202–12205
Chen W, Lei T, Qian T, Lv W, He W, Wu C, Liu X, Liu J, Chen B, Yan C, Xiong J (2018) A new hydrophilic binder enabling strongly anchoring polysulfides for high-performance sulfur electrodes in lithium-sulfur battery. Adv Energy Mater 8:1702889
Chen Q, Sun S, Zhai T, Yang M, Zhao X, Xia H (2018) Yolk-Shell NiS2 Nanoparticle-embedded carbon fibers for flexible fiber-shaped sodium battery. Adv Energy Mater 8:1800054
Chen W, Zhang X, Mi L, Liu C, Zhang J, Cui S, Feng X, Cao Y, Shen C (2019) High-performance flexible freestanding anode with hierarchical 3D carbon-networks/Fe7S8/graphene for applicable sodium-ion batteries. Adv Mater 31:1806664
Li P, Jeong JY, Jin BJ, Zhang K, Park JH (2018) Vertically oriented MoS2 with spatially controlled geometry on nitrogenous graphene sheets for high-performance sodium-ion batteries. Adv Energy Mater 8:1703300
Chen Z, Wu R, Liu M, Wang H, Xu H, Guo Y, Song Y, Fang F, Yu X, Sun D (2017) General synthesis of dual carbon-confined metal sulfides quantum dots toward high-performance anodes for sodium-ion batteries. Adv Funct Mater 27:1702046
Hu X, Jia J, Wang G, Chen J, Zhan H, Wen Z (2018) Reliable and general route to inverse opal structured nanohybrids of carbon-confined transition metal sulfides quantum dots for high-performance sodium storage. Adv Energy Mater 8:1801452
Li S, Ge P, Jiang F, Shuai H, Xu W, Jiang Y, Zhang Y, Hu J, Hou H, Ji X (2018) The advance of nickel-cobalt-sulfide as ultra-fast/high sodium storage materials: the influences of morphology structure, phase evolution and interface property. Energy Storage Materials 16:267–280
Xu X, Zeng H, Han D, Qiao K, Xing W, Rood MJ, Yan Z (2018) Nitrogen and sulfur co-doped graphene nanosheets to improve anode materials for sodium-ion batteries. ACS Appl Mater Interfaces 10:37172–37180
Guo Q, Ma Y, Chen T, Xia Q, Yang M, Xia H, Yu Y (2017) Cobalt sulfide quantum dot embedded N/S-doped carbon nanosheets with superior reversibility and rate capability for sodium-ion batteries. ACS Nano 11:12658–12667
Pan Y, Cheng X, Gong L, Shi L, Zhang H (2018) Nanoflower-like N-doped C/CoS2 as high-performance anode materials for Na-ion batteries. Nanoscale. 10:20813–20820
Zhang YH, Wang NN, Xue P, Liu YL, Tang B, Bai ZC, Dou SX (2018) Co9S8@carbon nanospheres as high-performance anodes for sodium ion battery. Chem Eng J 343:512–519
Yin M, Feng X, Zhao D, Zhao Y, Li H, Zhou W, Liu H, Bai X, Wang H, Feng C, Jiao Q (2019) Hierarchical Co9S8@Carbon hollow microspheres as an anode for sodium ion batteries with ultralong cycling stability. ACS Sustain Chem Eng 7:6122–6130
Pan Y, Cheng X, Gong L, Shi L, Zhou T, Deng Y, Zhang H (2018) Double-morphology CoS2 anchored on N-doped multichannel carbon nanofibers as high-performance anode materials for Na-ion batteries. ACS Appl Mater Interfaces 10:31441–31451
Wang Y, Zhang Y, Shi J, Kong X, Cao X, Liang S, Cao G, Pan A (2019) Tin sulfide nanoparticles embedded in sulfur and nitrogen dual-doped mesoporous carbon fibers as high-performance anodes with battery-capacitive sodium storage. Energy Storage Materials 18:366–374
Song Y, Bai S, Zhu L, Zhao M, Han D, Jiang S, Zhou YN (2018) Tuning pseudocapacitance via C-S bonding in WS2 nanorods anchored on N,S codoped graphene for high-power lithium batteries. ACS Appl Mater Interfaces 10:13606–13613
Wu F, Dong R, Bai Y, Li Y, Chen G, Wang Z, Wu C (2018) Phosphorus-doped hard carbon nanofibers prepared by electrospinning as an anode in sodium-ion batteries. ACS Appl Mater Interfaces 10:21335–21342
Chen C, Yang Y, Ding S, Wei Z, Tang X, Li P, Wang T, Cao G, Zhang M (2018) S-doped carbon@TiO 2 to store Li + /Na + with high capacity and long life-time. Energy Storage Materials 13:215–222
Lei T, Chen W, Lv W, Huang J, Zhu J, Chu J, Yan C, Wu C, Yan Y, He W, Xiong J, Li Y, Yan C, Goodenough JB, Duan X (2018) Inhibiting polysulfide shuttling with a graphene composite separator for highly robust lithium-sulfur batteries. Joule. 2:2091–2104
Chen W, Lei T, Lv W, Hu Y, Yan Y, Jiao Y, He W, Li Z, Yan C, Xiong J (2018) Atomic interlamellar ion path in high sulfur content lithium-montmorillonite host enables high-rate and stable lithium-Sulfur Battery. Adv Mater 30:1804084
Qiu W, Jiao J, Xia J, Zhong H, Chen L (2015) A self-standing and flexible electrode of yolk-shell CoS2 spheres encapsulated with nitrogen-doped graphene for high-performance lithium-ion batteries. Chemistry. 21:4359–4367
Zhong M-e, Guan J, Sun J, Guo H, Xiao Z, Zhou N, Gui Q, Gong D (2019) Carbon nanodot-decorated alveolate N, O, S tridoped hierarchical porous carbon as efficient electrocatalysis of polysulfide conversion for lithium-sulfur batteries. Electrochim Acta 299:600–609
Wu LL, Wang QS, Li J, Long Y, Liu Y, Song SY, Zhang HJ (2018) Co9 S8 nanoparticles-embedded N/S-codoped carbon nanofibers derived from metal-organic framework-wrapped CdS nanowires for efficient oxygen evolution reaction. Small. 14:e1704035
Ren J, Zhou Y, Xia L, Zheng Q, Liao J, Long E, Xie F, Xu C, Lin D (2018) Rational design of a multidimensional N-doped porous carbon/MoS2/CNT nano-architecture hybrid for high performance lithium–sulfur batteries. J Mater Chem A 6:13835–13847
Liu X, Liu H, Zhao Y, Dong Y, Fan Q, Kuang Q (2016) Synthesis of the carbon-coated nanoparticle Co9S8 and its electrochemical performance as an anode material for sodium-ion batteries. Langmuir. 32:12593–12602
Pan YL, Cheng XD, Gong LL, Shi L, Deng YR, Zhang HP (2018) Highly reversible Na ion storage in N-doped polyhedral carbon-coated transition-metal chalcogenides by optimizing the nanostructure and surface engineering. J Mater Chem A 6:18967–18978
Chen C, Wen Y, Hu X, Ji X, Yan M, Mai L, Hu P, Shan B, Huang Y (2015) Na+ intercalation pseudocapacitance in graphene-coupled titanium oxide enabling ultra-fast sodium storage and long-term cycling. Nat Commun 6:6929
Chen J, Zou G, Hou H, Zhang Y, Huang Z, Ji X (2016) Pinecone-like hierarchical anatase TiO2 bonded with carbon enabling ultrahigh cycling rates for sodium storage. J Mater Chem A 4:12591–12601
This research was funded by the National Natural Science Foundation of China Program (no. 51602111); the Natural Science Foundation of Guangdong Province (2018A030313739); Cultivation project of National Engineering Technology Center (2017B090903008); Xijiang R&D Team (X.W.), Guangdong Provincial Grant (2017A050506009); Special Fund Project of Science and Technology Application in Guangdong (2017B020240002); and 111 projects.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Preparation process of Co9S8@NSC. Figure S1. BJH pore width distribution of Co9S8@NSC (a) and NSC (b). Figure S2. N 1 s XPS spectra of Co9S8@NSC. Figure S3. (a-c) SEM and (d-f) TEM of NSC at different magnification. (The inset of (f) is the SAED of NSC.) Figure S4. EDS mapping of Co9S8@NSC. Figure S5. (a) CV curves of NSC with different cycles at 0.1 mV s-1; (b) Charge-discharge profiles of NSC at various cycles at 200 mA g-1. Figure S6. (a) Nyquist plots of Co9S8@NSC and (b) NSC before and after cycles; EIS curves comparison between Co9S8@NSC and NSC for initial (c), 5 cycles later (d) and 10 cycles later (e). Figure S7. The linear relation between Ip and v1/2 according to the Randles-Sevick equation.
About this article
Cite this article
Zhang, X., Shang, C., Wang, X. et al. Double Morphology of Co9S8 Coated by N, S Co-doped Carbon as Efficient Anode Materials for Sodium-Ion Batteries. Nanoscale Res Lett 15, 19 (2020). https://doi.org/10.1186/s11671-020-3256-8
- N, S co-doping
- Rate performance
- Node materials